Ternary Systems: Review A ternary temperature-composition “phase diagram” at constant total pressure may be plotted as a threedimensional “space model” within a right triangular prism with the equilateral composition triangle (……… triangle) as base and temperature as vertical axis. Outline • Ternary Phase Diagram: - Review - Alkemade’s Lines - Crystallization Path Analysis • Vertical Sections • Isothermal Sections • The three binary subsystems such as A-B, B-C, and C-A, can be seen on the vertical faces of the prism. The three binary eutectic points are e1, e2, and e3. • Within the prism, the three liquidus surfaces descending from the melting points of pure A, B, and C and make the ternary eutectic point E. Mech 6661 lecture 11/1 Mech. Eng. Dept. - Concordia University Dr. M. Medraj Dr. M. Medraj Ternary Systems: Review The lines on the liquid surface are the constant temperature lines called isotherms. e2 Temperature T2 T3 T4 T5 e2 T6 T7 T8 e1 • e3 • e3 T6 T7 T8 • T5 MA C T1 E E • B e1 A The plan view of the ternary space model with the important points Dr. M. Medraj Space model for a simple eutectic ternary system A-B-C Mech 6661 lecture 11/2 Mech. Eng. Dept. - Concordia University Alkemade lines are the lines that connect the primary compositions of two phase fields which share a common boundary. Alkemade lines divide a phase diagram into compatibility triangles. This diagram is divided into two compatibility triangles: A-C-AB and B-C-AB. Alkemade’s theorem can be used to determine the direction of decreasing temperature on a phase diagram, as we will discuss later. Mech 6661 lecture 11/3 C C A B AB A B AB Each boundary line on the diagram has an Alkemades line associated with it. Space model for a simple eutectic ternary system A-B-C Mech. Eng. Dept. - Concordia University B A MC T1 T2 T3 T4 MB T T Alkemade Lines T T C Dr. M. Medraj Mech. Eng. Dept. - Concordia University Mech 6661 lecture 11/4 Alkemade Lines: Ternary Invariant Points • The intersection of a boundary line (or extended boundary line) with its corresponding Alkemade line (or extended Alkemade line) is a maximum in temperature on the boundary line and a minimum in temperature on the Alkemade line. This point is labeled “m”. • This theorem can be used to draw arrows on the diagram showing the direction of decreasing temperature. • The “m” on the triangle edges are the binary invariant points – ……….. points in this example • The point that resulted from the intersection of AB-C Alkemede line and the boundary between C and AB is called ……….. point. • E1 and E2 are ternary eutectic points. Dr. M. Medraj Alkemade Lines: Ternary Invariant Points C C •The Alkemade line between C and AB, in this diagram, does not cross the boundary line that its end components share. A • First draw an extension of the boundary line so that it will intersect the Alkemade line. B AB A B AB Ternary system with a ………. binary compound Mech 6661 lecture 11/5 Mech. Eng. Dept. - Concordia University Alkemade Lines: Ternary Congruent Compound • As usual, we begin by highlighting each boundary line and the Alkemade line associated with it. • Identify the compatibility triangles. • Label the max/min points. • Draw the temperature arrows on the boundary and Alkemade lines. C A ABC points are labeled. A B B • The diagram is finished. Ternary system with a congruent ternary compound Dr. M. Medraj Mech. Eng. Dept. - Concordia University Dr. M. Medraj B AB A AB B Ternary system with a ………….. binary compound Mech 6661 lecture 11/6 Mech. Eng. Dept. - Concordia University • As usual, we begin by highlighting each boundary line and the Alkemade line associated with it. • Identify the compatibility triangles. • Label the max/min points. • Draw the temperature arrows on the boundary and Alkemade lines. C • And the ternary invariant • Then use the intersection point where the lines meet as a guide for drawing the temperature arrows. The temperature arrows on the Alkemade line will go towards the intersection point. A Alkemade Lines: Ternary Incongruent Compound • The binary invariant points are given their appropriate labels. C • This phase diagram is also divided to two compatibility triangles. C Mech 6661 lecture 11/7 C C The ABC/A,B,C boundary lines and the associated Alkemade lines ……….. cross. To correct for this, draw a temporary extension of the ABC-C Alkemade line and of ABC/A and B boundaries . • The binary invariant points are given their appropriate labels. • And the ternary invariant points are labeled. • The diagram is finished. Dr. M. Medraj A ABC ABC B A B Ternary system with a incongruent ternary compound Mech. Eng. Dept. - Concordia University Mech 6661 lecture 11/8 Crystallization Path Analysis Crystallization Path Analysis A • First, identify the compounds on the diagram and their corresponding primary crystallization fields. • Then connect compounds, whose primary crystallization fields share a boundary, with Alkemade lines. AC A • First locate the composition of interest (co) on the diagram. a • Identify the compatibility triangle: in our example, it is AC – B–C • Remember that where Alkemade lines cross boundary lines the boundary lines are at a local maximum and the Alkemade lines are at a local minimum in temperature B Mech 6661 lecture 11/9 Dr. M. Medraj Crystallization Path Analysis A • The crystallization path begins at the point and moves away from the the primary phase as B begins to crystallize out of the composition. a • Finally, at the ternary invariant point all of the remaining liquid crystallizes. Dr. M. Medraj C Mech 6661 lecture 11/10 Mech. Eng. Dept. - Concordia University Isothermal sections in ternary phase diagrams are horizontal slices through the three dimensional diagram. All points on the section are at the same temperature, unlike the normal view of the ternary diagram where the liquidus surface is seen. ac b Mech. Eng. Dept. - Concordia University c Ternary Isothermal Sections AC B b co c C Mech 6661 lecture 11/11 A Ternary diagram is a flat representation of the curved liquidus surface. Therefore, in a normal ternary diagram, everything shown is liquid. In an isothermal section both liquid and solid can be present. Dr. M. Medraj Temperature • Now draw a tie line from the primary phase B through the point to the boundary with ac. ac • And final liquid composition: The final liquid composition is the ternary invariant point where all three compounds in the B compatibility triangle meet. C Mech. Eng. Dept. - Concordia University • Now AC begins to crystallize out as the path follows the boundary line to its ternary invariant point. AC • Next determine its primary crystallization field. • The Alkemade lines form compatibility triangles. Dr. M. Medraj • Now we are ready to trace the cooling path of any ternary composition. T = value B A Mech. Eng. Dept. - Concordia University C Mech 6661 lecture 11/12 CaF2-LiF-MgF2 Isothermal Section at 1100°C LiF-RbF-BeF2 Isothermal Section at 700°C • Identify and trace all of the isotherms for the temperature for isothermal section of 1100oC. • • Then fill in for the region of the diagram where the liquidus area is still below the temperature of 1100°C. Trace all isotherms on this diagram at 700°C, and draw the tie lines. Every phase field left at this point will consist of three phases. There will either be two solids and a liquid of a specific composition, or there will be three solid phases. Two phase regions occur when the intersection between the isotherm and a single phase region (e.g. liquid) is a line (not a point). • Draw both lines that intersect with the phase boundary line and surround the two-phase region. The three phase region shown here consists of Rb2BeF4 – Rb3BeF5 – L1. • Finally, draw in dashed tie lines from the composition to the liquidus region of 1100oC. Dr. M. Medraj Mech. Eng. Dept. - Concordia University Mech 6661 lecture 11/13 There are 4 types of phase fields in the isothermal section of a ternary system: – The single phase region. The phase can be a liquid or a solid solution. Liquid is more common. In the previous examples, this region is composed entirely of a liquid of varying composition. – The two Phase region, containing both solid and liquid. The composition of the liquid is found using the tie lines that were drawn in on the second slide. The solid is of a single, unvarying composition. This region shares a border with the liquid region. Remember that the regions with one corner in contact with the liquidus have liquid in them with the comp. of the contact point. The remaining portion has either three solids, or a liquid and two solids. •Trace all Alkemade lines that do not come into contact with the liquidus lines, or cross any of the tie lines. • Everything that is left is all ……. (three-……….. region). None that the previous examples do not contain all four types of phase fields. Therefore the next example will be at 400°C. Mech 6661 lecture 11/15 Trace all isotherms on this diagram at 400°C, identify the liquid and draw the tie lines in the two phase regions. • Identify all the regions that contain ……... – The solid region, contains three distinct solids. This region is triangular, and has no contact with the liquid region. Mech. Eng. Dept. - Concordia University • Liquid – The three Phase region, composed of two solid compositions and one unvarying liquid composition. This region is easily recognized by its sole point of contact with the liquid region, labeled L1 in the previous slide. Dr. M. Medraj Mech 6661 lecture 11/14 Three-Phase Regions LiF-RbF-BeF2 Isothermal Section at 400°C Ternary Isothermal Sections • Mech. Eng. Dept. - Concordia University Dr. M. Medraj Dr. M. Medraj Mech. Eng. Dept. - Concordia University Mech 6661 lecture 11/16 LiF-RbF-BeF2 Isothermal Section at 400°C Liquid and two solids regions: Liquid L1 A I II B L L2 L3 4 D A) L1 & Li2BeF4 & Li2RbBe2F7 B) L2 & Li2RbBeF7 & LiRbBeF4 C) L3 & LiRbBeF4 & Rb2BeF4 D) L4 & RbBrF3 & Rb2BeF4 10 minutes Break Three solids regions : I) LiF & Li2RbBe2F7 & Li2BeF4 C II) LiF & RbBe2F7 & LiRbBeF4 III V IV III) LiF & Rb2BeF4 & LiRbBeF4 IV) LiF & Rb2BeF4 & Rb3BeF3 VI V) LiF & LiRbF2 & Rb3BeF5 VI) RbF & LiRbF2 & Rb3BeF5 Dr. M. Medraj Mech 6661 lecture 11/17 Mech. Eng. Dept. - Concordia University Mech. Eng. Dept. - Concordia University Dr. M. Medraj Ternary Vertical Sections: Introduction Constructing Vertical Sections • Vertical sections are two dimensional representations of the crystallization paths for a series of points that lie along a chosen line on a ternary phase diagram. • Draw Alchemades lines • Identify direction of falling temperature on boundary lines. C ZrO2 ZrTiO4 E ZrTiO4 T 1610° 1590° 1580° B Dr. M. Medraj • Identify primary phase fields ZrO2 • There are three main lines in a vertical section which divide the various solids and liquid phases. These three lines are called the liquidus, subliquidus, and solidus lines, and will be explained in more detail later. Vertical sections in ternary systems can be very complicated due to the crossing of Alkemedes’ lines and changing crystallization paths. Mech 6661 lecture 11/18 Al2O3 TiO2 Al2TiO5 A Space model for a simple eutectic ternary system A-B-C Mech. Eng. Dept. - Concordia University Mech 6661 lecture 11/19 TiO2 Al2TiO5 Dr. M. Medraj Al2O3 Mech. Eng. Dept. - Concordia University Mech 6661 lecture 11/20 Constructing Vertical Sections Constructing Vertical Sections Step 1 - Solidus lines • Which compatibility triangles are crossed? • Choose the section line (x - y). • Draw diagram framework. ZrO2 • Find the associated ternary invariant points. ZrO2 • Indicate temperatures on (x - y) diagram. • Draw Solidus lines on (x - y) diagram. ZrTiO4 ZrO2 ZrO2 x 1590° 1610° 1590° ZrTiO4 ZrTiO4 ZrTiO4 1610° y 1610° 1580° 1580° Al2O3 TiO2 Al2TiO5 TiO2 TiO2 Al2O3 Al2TiO5 x y Mech. Eng. Dept. - Concordia University Dr. M. Medraj Mech 6661 lecture 11/21 TiO2 Dr. M. Medraj ZrO2 ZrO2 x 1590° ZrTiO4 TiO2 TiO2 Mech 6661 lecture 11/22 • These compositions separate regions of similar crystallization paths. Therefore, the crystallization paths of these compositions directly intersect important features of the ternary diagram. Some examples of these features are given. Examples: y Ternary Invariant Points 1610° m – Points 1590° 1580° Alchemades Lines Diagram Boarders Al2TiO5 Al2TiO5 Mech. Eng. Dept. - Concordia University y • The essential compositions used to develop the sub-liquidus line in a vertical section are called important compositions. The purpose of these important compositions is to reduce the work load on the investigator. 1610° Al2O3 x - Liquidus line • The top view of the liquidus line can be seen on the ternary diagram. • Find the end points and points where the liquidus line crosses any boundary lines. 1580° Al2O3 Vertical Section: Important Compositions • Estimate and plot relative temperatures of these points. • Draw liquidus line - estimate curvature. ZrTiO4 1590° 1580° Al2TiO5 Al2TiO5 Constructing Vertical Sections Step 2 Al2O3 Al2O3 x y Now we must Find and indicate all of the important compositions. Dr. M. Medraj Mech. Eng. Dept. - Concordia University Mech 6661 lecture 11/23 Dr. M. Medraj Mech. Eng. Dept. - Concordia University Mech 6661 lecture 11/24 Constructing Vertical Sections Constructing Vertical Sections Step 4 - Alchemades line Intersection Step 3 - Sub-liquidus line ZrO2 ZrTiO4 ZrO2 x 1590° ZrTiO4 • Find and indicate all of the important compositions. • Perform isoplethal analysis - record temperature where boundary line is intersected. • Draw sub-liquidus line. • Check each segment with an intermediate isoplethal analysis. • Find and indicate all compositions where section line crosses an alchemades line. • Perform isoplethal analysis and plot final crystallization temperature. ZrO2 • Draw lines which indicate material is all solid ZrTiO4 ZrO2 x 1590° 1610° y 1580° ZrTiO4 1610° y 1610° 1580° Al2TiO5 TiO2 TiO2 Al2O3 Al2TiO5 x Al2O3 1590° 1580° Al2TiO5 y TiO2 Mech 6661 lecture 11/25 Mech. Eng. Dept. - Concordia University Dr. M. Medraj 1610° 1590° 1580° Al2O3 TiO2 Al2TiO5 Dr. M. Medraj Al2O3 x Mech. Eng. Dept. - Concordia University y Mech 6661 lecture 11/26 Constructing Vertical Sections Step 5 - Labels • Refer to the ternary diagram and label vertical section The End ………….. ………. Liq. + Al2TiO5 …………. Liq. TiO2 ZrTiO4 1610° ……… 1590° Liq. ZrTiO4 Al2TiO5 Liq. ZrO2 Al2TiO5 ……. …………… x Dr. M. Medraj THANK YOU VERY MUCH Liq. ZrO2 Al2O3 ZrO2 + Al2O3 + Al2TiO5 1580° TiO2 + ZrTiO4 + Al2TiO5 Liq. ZrO2 Al2TiO5 y Mech. Eng. Dept. - Concordia University Mech 6661 lecture 11/27 Dr. M. Medraj Mech. Eng. Dept. - Concordia University Mech 6661 lecture 11/28

© Copyright 2023 Paperzz